 gap [@Oostinga2008gii]. This is because electrical transport is extremely sensitive to defects and impurities, and a very high quality graphene is required to reach the intrinsic BLG behavior. Recent transport studies [@Xia2010gfe] however demonstrate transport gaps closer to those obtained through IR spectroscopy.

Electron-phonon coupling in gated BLG shows up in tunable electron-phonon Fano resonances [@Tang2010atp; @Kuzmenko2009gti; @Cappelluti2010psa]. There is a host of other effects that originate from unique gate-tunable electronic structure in BLG that have been predicted theoretically and are amenable to spectroscopic studies, e.g., a rich Landau level spectrum structure [@Zhang2011mcb]. However, we must leave this topic now to at least briefly discuss MLG.

The electronic structure of MLG has been investigated experimentally using optical spectroscopy. Figure \[fig:5.1.1\]a displays a set of IR absorption spectra from $L = 1$ to $8$ layer graphene over the photon-energy range of $0.2$–$0.9\,\text{eV}$ [@Mak2010teo]. At energies in the range $\gamma_1 \ll \hbar\omega \ll \gamma_0$ the MLG is expected to behave in the first approximation as a stack of uncoupled SLG, each possessing the universal optical conductivity $\sigma_0$, Eq. . Indeed, at energies above $0.8\,\text{eV}$, the measured optical absorption scales linearly with $L$. However, at lower energies, the absorption becomes highly structured and distinct for different $L$. The evolution of the absorption spectra as a function of $L$ can be visualized from the false color plot Fig. \[fig:5.1.1\]b in which the principle transition energies are marked by the solid curves. The shape of these curves can be understood through zone-folding of the graphite band-structure. In particular, a gapless band is present if $L$ is odd and absent if it is even [@Mak2010teo].

Outlook {#sec:outlook}
=======

A wealth of spectroscopic data analyzed in this review has provided a panoramic picture of electronic phenomena in graphene. The concept of 2D Dirac quasiparticles offers a unifying description of the gross features revealed in all spectroscopic and transport probes. At the same time,
gap [ @Oostinga2008gii ]. This is because electrical transport is extremely sensible to defect and impurities, and a very high timbre graphene is required to pass the intrinsic BLG behavior. late tape drive studies [ @Xia2010gfe ] however show transport gaps nearer to those obtained through IR spectroscopy. 

 Electron - phonon coupling in gated BLG shows up in tunable electron - phonon Fano rapport [ @Tang2010atp; @Kuzmenko2009gti; @Cappelluti2010psa ]. There is a server of other effects that originate from alone gate - tunable electronic structure in BLG that have been predicted theoretically and are amenable to spectroscopic studies, for example, a rich Landau level spectrum social organization [ @Zhang2011mcb ]. However, we must leave this subject now to at least briefly discuss MLG. 

 The electronic structure of MLG has been investigated experimentally using ocular spectroscopy. Figure   \[fig:5.1.1\]a displays a set of IR absorption spectra from $ L = 1 $ to $ 8 $ layer graphene over the photon - energy range of $ 0.2$–$0.9\,\text{eV}$ [ @Mak2010teo ]. At energies in the range $ \gamma_1 \ll \hbar\omega \ll \gamma_0 $ the MLG is expected to behave in the first approximation as a stack of uncoupled SLG, each possessing the universal ocular conductivity $ \sigma_0 $, Eq.  . Indeed, at energies above $ 0.8\,\text{eV}$, the careful optical absorption scales linearly with $ L$. However, at lower department of energy, the absorption becomes highly structured and distinct for unlike $ L$. The evolution of the absorption spectra as a function of $ L$ can be visualized from the false color plot Fig.   \[fig:5.1.1\]b in which the principle transition energies are marked by the solid curves. The form of these bend can be understood through zone - folding of the graphite band - structure. In particular, a gapless isthmus is present if $ L$ is odd and absent if it is even [ @Mak2010teo ]. 

 Outlook { # sec: outlook } 
 = = = = = = = 

 A wealth of spectroscopic datum analyzed in this follow-up has provided a panoramic video of electronic phenomena in graphene. The concept of 2D Dirac quasiparticle offers a unifying description of the gross features revealed in all spectroscopic and conveyance probes. At the like time,
 gao [@Oostinga2008gii]. This is begause electrical transpmrt is extremeuy sensitive to defects and mmpueitiew, and a very high qualkty graphvne is rewuirtd to reach the iifrinsic BLG bsmaviox. Cecent transporj studies [@Xid2010gfe] however damundtrate transport gaps closer to thofe obtaonfd through IR fpecurofcopg.

Vltctron-phonon coupling in gated BLF shows up in tunablr electron-phonon Fano resojancfs [@Tang2010atp; @Kuzmenkl2009gti; @Cappelouti2010[wa]. There is x host of other effecta that originate from unique gage-tuncble electrinuc djructure in ULG thwt have been predictad theotetically and sre amwnable to spectroscopmc studies, e.g., a rich Landau lavzl spectrum structure [@Zyang2011mwb]. Hmwevde, wd mhsv lsave tjis topic now to at leasr briefly discuss MKG.

Eye electronic struceuwe of MLG has been investigated experimtntalmy using optical spectriscopy. Figure \[fig:5.1.1\]a disklays a see of IR absorption spectra from $L = 1$ to $8$ layer gra[hene uvex the oyohon-energy range of $0.2$–$0.9\,\text{eV}$ [@Mak2010teo]. At energies yh uhe range $\gamma_1 \lj \hbar\omega \lp \bwmma_0$ the MLG ks expzdtsd to behave in thf first appriximation as s stack of uncoupled SLG, eaxh possessiny tye universal opticcl conductivnty $\sibma_0$, Ea. . Indeed, at energies abuve $0.8\,\fext{eV}$, the leasured kotical absorptiov sbalev linearly with $L$. However, wt lower xnergnes, the xbsotption fecomes hihhly structured and distlnct yor dhfferent $L$. The evolution of the absorptioi spectra as s xunbtion of $J$ can be visualizeq from the falxe colox plot Fig. \[fig:5.1.1\]b ih which the princi[le transitiot energies arx marked fy tye silid cufxes. The shape pf these buxves can ve understood thromgh zuhe-folding of thz traphite band-sttucgurq. Pn 'artisglar, a gaplevs bxnd os prdsent if $L$ ls udd snd absent if it is aven [@Mak2010teo].

Outlook {#sec:publook}
=======

A weqlth of fpectroscopic data analyzed in uhis rxview ias prpviqed a panoramic picture of eledtronic pjenjmena in gra[henc. Thg concept oy 2D Dirac quasiparticles offers a unifyiig description of the geoss features reveaktd in all spertroscjpic and dransport probes. At rhe same time,
gap [@Oostinga2008gii]. This is because electrical transport sensitive defects and and a very to the intrinsic BLG Recent transport studies however demonstrate transport gaps closer to obtained through IR spectroscopy. Electron-phonon coupling in gated BLG shows up in tunable Fano resonances [@Tang2010atp; @Kuzmenko2009gti; @Cappelluti2010psa]. There is a host of other effects that from gate-tunable structure BLG that have been predicted theoretically and are amenable to spectroscopic studies, e.g., a rich Landau spectrum structure [@Zhang2011mcb]. However, we must leave this now to at least discuss MLG. The electronic structure MLG been investigated using spectroscopy. \[fig:5.1.1\]a displays a of IR absorption spectra from $L = 1$ to $8$ layer graphene over the photon-energy range of [@Mak2010teo]. At the range \ll \ll the MLG is behave in the first approximation as uncoupled SLG, each possessing the universal optical conductivity Eq. . at energies above $0.8\,\text{eV}$, the measured absorption scales linearly with $L$. However, at lower the absorption becomes highly structured and distinct for different $L$. The evolution of the absorption a function of $L$ be visualized from false plot \[fig:5.1.1\]b which the transition energies are marked by the solid curves. The shape of curves can be understood through zone-folding of the graphite band-structure. a band is present $L$ is odd and if is even [@Mak2010teo]. Outlook A of in review provided a panoramic picture electronic phenomena in graphene. The of 2D Dirac quasiparticles the gross features revealed in all spectroscopic and probes. At the same time,
 gap [@Oostinga2008gii]. This is becauSe electricAl traNspOrt Is ExtrEmelY sensitive to deFEcts And impurities, and a very hIgh quAlITy grAPhEne is RequireD To REAch ThE iNtrInSIc bLG beHavIor. ReceNt transporT stUdIes [@Xia2010gfe] howEVeR demonstraTe tRansport gaps CloSer to tHoSe oBTaineD thRough iR specTRoscopY.

Electron-PhONon couPLing in gATEd bLG sHows up in tunable elECtROn-phonon Fano reSonancEs [@tAnG2010ATp; @KUzmEnko2009gti; @CapPeLluti2010PSa]. There IS a HOST of OTher effects thAt originate FRom Unique GaTe-tUNable eLectrOnIC stRucture in BLg thaT have been PredicTEd theorETically And are AmeNabLe to SPeCtRosCoPIc sTUdIes, E.G., a rIch LandaU lEvEl speCtruM STRUctuRe [@ZHang2011Mcb]. HoWever, we must leAve This TOpiC now tO at leAst bRiEfly dIscuss mLG.

ThE eLectronic structUre oF MLG has beEn iNvEstIgAted eXPerimeNtaLly Using opTical spECtrOsCOPY. FIgure \[fig:5.1.1\]a displays a SeT OF Ir absorptIon speCTrA fROm $L = 1$ to $8$ layEr GraPhenE OVer thE phoTOn-Energy raNge of $0.2$–$0.9\,\tEXt{EV}$ [@mak2010teo]. AT eNergieS iN thE raNge $\gaMMa_1 \ll \Hbar\omEga \ll \gamMa_0$ the mlG is expected to BEhave in the firST aPPRoXImatIon As a stack of uNcouPLed SlG, eaCH pOssESsing The unIvERsAL optical conductivitY $\sIgma_0$, Eq. . indeeD, at energies abOve $0.8\,\text{eV}$, tHE MEasured oPticAL aBSorption scales LineaRly with $L$. HoWEver, at loWer enErgies, thE absorptiON Becomes hIghLy sTruCtuRED aNd distinct for DIFferEnT $L$. The evOluTion of tHe aBsoRptIon SpEctra as a fUnction oF $L$ CaN bE vIsuAlizeD From the fAlSe cOlOr pLot FiG. \[Fig:5.1.1\]b in Which The pRiNcIPle TransitIOn ENErgiEs ArE marKed By The soLid cURveS. The shaPe of these CurVEs caN bE uNderstoOd through zone-FoLding of the GrAphIte banD-STructure. in particular, a gapless banD Is preseNt iF $L$ is oDd anD absent if It iS even [@MAk2010tEO].

OutloOk {#sec:oUtlooK}
=======

A WeaLTH of spECTrOscOpIc data analYZEd iN this ReView Has provIded a panoramic pictURe oF electronic phEnoMena IN GrAphENe. tHe cOnCEpt OF 2d Dirac quasipartIcles offerS a UNiFying descrIPtiOn Of the grOss featUres rEVealed iN all spectRoscopic aNd TranSPOrt Probes. At thE same timE,
 gap [@Oostinga2008gii]. T his is bec auseele ctr ic al t rans port is extrem e ly s ensitive to defects an d imp ur i ties ,  a nd avery hi g hq u ali ty  g rap he n eis re qui red toreach theint ri nsic BLG beh a vi or. Recent  tr ansport stud ies  [@Xia 20 10g f e] ho wev er de monstr a te tra nsport ga ps closer to thos e ob tain ed through IR spe c tr o scopy.

Electr on-pho no n  c o u pli ngin gated B LG  show s  up int un a b l e e l ectron-phonon  Fano reson a nce s [@Ta ng 201 0 atp; @ Kuzme nk o 200 9gti; @Capp ellu ti2010psa ]. The r e is ah ost ofothereff ect s th a tor igi na t e f r om  un i que  gate-tu na bl e ele ctro n i c stru ctu re i n BLG  that have be enpred i cte d the oreti call yand a re ame nable  t o spectroscopic  stu dies, e.g .,aric hLanda u  level  sp ect rum str ucture[ @Zh an g 2 0 11 mcb]. However, wemu s t  l eave thi s topi c  n ow to at le as t b rief l y  disc ussM LG .

The e lectro n ic  s tructur eof MLG  h asbee n inv e stig ated e xperimen tally using opticals pectroscopy.F ig u r e\ [fig :5. 1.1\]a disp lays a se t of IR  ab s orpti on sp ec t ra from $L = 1$ to $8$  l ayer g raphe ne over the p hoton-ener g y range of  $0. 2 $– $ 0.9\,\text{eV} $ [@M ak2010teo] .  At ener giesin the r ange $\ga m m a_1 \ll\hb ar\ ome ga\ l l\gamma_0$ the M LG i sexpecte d t o behav e i n t hefir st  approxim ation as  a  s ta ck  of  unco u pled SLG ,eac hpos sessi n g theunive rsal  o pt i cal  conduc t iv i t y $\ si gm a_0$ , E q.  . In deed ,  at  energi es above$0. 8 \,\t ex t{ eV}$, t he measured o pt ical absor pt ion  scale s linearly  with $L$. However, atl ower en erg ies,theabsorptio n b ecomes  hi g hly st ructur ed an ddis t i nct f o r  d iff er ent $L$. T h e  ev oluti on  ofthe abs orption spectra as a f unction of $L $ c an b e vi sua l iz e d f ro m  th e false color plo t Fig. \[f ig : 5. 1.1\]b inw hic hthe pri ncipletrans i tion en ergies ar e markedby  the s oli d curves.The shap e of thes e  curv e scan b e u nderst oo d t hroug h zone - fol dingof the  g raphit e ban d- structur e. In particular, a gap less b and i s p resent if  $L $  is  odd andabse nt if it i s e ven  [@Ma k20 1 0teo] .

O u tl ook {#sec :out l ook}
==== = == 

A w ea lth of spec t r o sco pic d ata analyz ed i n this review has provided a pan oram i c  pi ctu r e of  e lectronic phen ome na i n graphe ne . The conce pt of 2D  D i rac q uasipa rticle s offer s au nifyin g de scr iption of  th eg ross fe at ur e s reve aled  i n allspectr o scop i c  and transport p robes . At th e  sa me ti me ,
 gap_[@Oostinga2008gii]. This_is because electrical transport_is extremely_sensitive_to defects_and_impurities, and a_very high quality_graphene is required to_reach the intrinsic_BLG_behavior. Recent transport studies [@Xia2010gfe] however demonstrate transport gaps closer to those obtained through_IR_spectroscopy.

Electron-phonon coupling_in_gated_BLG shows up in tunable_electron-phonon Fano resonances [@Tang2010atp; @Kuzmenko2009gti;_@Cappelluti2010psa]. There_is a host of other effects that originate_from_unique gate-tunable electronic_structure in BLG that have been predicted theoretically and_are amenable to spectroscopic studies, e.g.,_a rich Landau_level_spectrum_structure [@Zhang2011mcb]. However, we_must leave this topic now to_at least briefly discuss MLG.

The electronic_structure of MLG has been investigated experimentally_using optical spectroscopy. Figure \[fig:5.1.1\]a displays a_set of IR absorption spectra_from $L_= 1$ to $8$ layer_graphene over the_photon-energy range_of $0.2$–$0.9\,\text{eV}$ [@Mak2010teo]._At energies in the range $\gamma_1_\ll \hbar\omega \ll_\gamma_0$ the MLG is expected to_behave_in the first_approximation_as_a stack_of uncoupled SLG,_each_possessing the_universal_optical conductivity $\sigma_0$, Eq. . Indeed, at_energies_above $0.8\,\text{eV}$, the measured optical absorption scales_linearly with $L$. However,_at_lower energies, the absorption_becomes highly structured and distinct_for different $L$. The evolution of_the absorption_spectra as_a function of $L$ can be visualized from the false color_plot Fig. \[fig:5.1.1\]b in which the principle_transition energies are marked_by the_solid_curves. The shape_of_these curves_can be understood through zone-folding of the_graphite band-structure._In particular, a gapless band is_present if $L$ is_odd_and absent if it is even_[@Mak2010teo].

Outlook {#sec:outlook}
=======

A wealth of spectroscopic data_analyzed in this review has_provided_a_panoramic picture of electronic phenomena_in graphene. The concept of 2D_Dirac quasiparticles offers_a unifying description of the gross features_revealed_in all spectroscopic and transport probes._At_the same time,